**Microscopic quantum theory of spatially resolved photoluminescence** **in semiconductor quantum structures**

G. Pistone,^{a)}S. Savasta, O. Di Stefano, and R. Girlanda

*Istituto Nazionale per la Fisica della Materia INFM and Dipartimento di Fisica della Materia e Tecnologie*
*Fisiche Avanzate, Universita` di Messina, Salita Sperone 31, I-98166 Messina, Italy*

We present a microscopic analysis of spatially resolved photoluminescence and photoluminescence excitation spectroscopy in semiconductor quantum structures. Such theoretical and numerical framework provides a general basis for the description of spectroscopic imaging in which the excitation and detection energies and spatial positions can all independently be scanned. The numerical results clarify the impact of the near-field optical setup on the obtained images and resolutions. 关DOI: 10.1063/1.1711184兴

In recent years, measurements based on spatially re-
solved photoluminescence 共PL兲 provided direct information
on the spatial and energy distribution of light emitting nano-
metric centers of semiconductor quantum structures, thus
opening a rich area of physics involving spatially resolved
quantum systems in a complex solid state environment.^{1– 6}In
particular, near-field optical microscopy and spectroscopy
can detect the optical characteristics of individual quantum
dots共QDs兲 among, e.g., a high-density ensemble of naturally
formed QDs,^{7} whereas usual far-field methods provide only
ensemble-averaged properties. Detailed simulations of Zim-
mermann, Runge, and Savona^{8,9}have clarified many aspects
of the intrigued nonequilibrium dynamics giving rise to pho-
toluminescence spectra in these quantum structures. How-
ever, theoretical simulations of near-field imaging spectros-
copy of semiconductor quantum structures focus on calcu-
lations of local absorption.^{10–13} In contrast, as a matter of
fact, almost all experimental images are obtained from PL
measurements. Here we present a microscopic theory of
spatially resolved photoluminescence in quantum structures
that includes both light quantization 共essential to describe
radiative recombination兲 and phonon scattering. The theory
also includes the description of spatially confined excitation
共illumination mode兲 and/or detection 共collection mode兲. It is
worth noting that we are faced with a strictly nonequilibrium
problem. Nonequilibrium here arising from both radiative
recombination 共preventing full thermalization兲 and from the
local nature of the excitation source 共in the illumination-
mode setup兲. We are also faced with the problem of the dif-
*ferences between illumination (I) and collection (C) scan-*
ning near-field optical microscopy共SNOM兲 instruments. The
equivalence between these two working modes has been
established on the basis of the reciprocity theorem for elec-
tromagnetic fields.^{14} However, this theorem holds for linear
and passive media. While semiconductor structures, at low
excitation densities, show a linear behavior, phonon scatter-
ing and radiative recombination prevent them from being
passive.

The positive frequency components of the operator de-

scribing the signal that can be detected by a general near-
field setup can be expressed as^{15}*Sˆ*_{t}^{⫹}*⫽Aˆ*bg⫹*⫹Sˆ*^{⫹}*, where Aˆ*

bg⫹ is
the elastic background signal 共largely uniform along the
*x – y plane*兲 proportional to the input electric-field operator,
*and Sˆ*^{⫹}is related to the sample polarization density operator
**Pˆ**⫹**(r): Sˆ**^{⫹}**⫽A兰drPˆ**^{⫹}**(r)•E**^{C}**(r), where***A is a complex con-*
**stant and E**_{C}**(r) is the signal mode delivered by the tip. Pho-**
toluminescence can be defined as the incoherent part of the
emitted light intensity.^{16} The PL that can be measured by a
photodetector after the collection setup 共broadband detec-
tion*兲 is proportional to I*PL*⫽I⫺I*coh⫽具^{Sˆ}^{⫺}^{(}^{)Sˆ}^{⫹}^{(}^{)}典

⫺兩具^{Sˆ}^{⫹}^{(}^{)}典兩^{2}. Analogously, the steady-state spectrum of in-
coherent light emitted by the semiconductor quantum struc-
ture and detected by the SNOM setup can be expressed as

*I共**C*兲⫽1

## 冕

0⬁

*d*具^{Sˆ}^{⫺}*共0兲Sˆ*^{⫹}共兲典^{e}^{i}^{}^{C}^{}^{.} ^{共1兲}

The interband polarization density operator can be expressed
**in terms of exciton operators as Pˆ**^{⫹}**(r)**⫽eh*f (z)*⌿_{␣}^{eh}(

**⫽0,R)Bˆ**_{␣}*, where e and h are appropriate sets of quantum*
numbers which label the carrier states involved in the optical
*transition. The operator Bˆ*

␣† creates an exciton state 共one
electron-hole pair*兲 Bˆ*_{␣}^{†}兩0典* ^{⬅兩E}*1,␣典

^{with}

^{energy}1,␣.

⌿_{␣}^{eh}(**,R) is the exciton wave function with**indicating the
**relative in-plane electron-hole eh coordinate and R describes**
*the center of mass motion, while f (z)⫽u**e**(z)u*_{h}*(z) is the*
product of the electron and hole envelope functions along the
confinement direction. If the disorder induced broadening is
small compared to the exciton binding energy, only the low-
*est bound state 1s at the fundamental sublevel transition has*
to be considered and the exciton wave function can be fac-
torized as ⌿_{␣}^{eh}(** ^{,R)}**⫽

*1s*(

^{)}␣

**(R).**

^{9}In the low-excitation

*regime the relation Bˆ*

_{␣}⯝兩0典具

*1,␣兩 can be assumed and it can*

^{E}*be shown that the operators Bˆ*

_{␣}behave as Boson operators.

^{17}Within these assumptions, the Hamiltonian determining the dynamics of the semiconductor system is given by the three contributions: the bare excitonic Hamiltonian of the semi- conductor system, the interaction Hamiltonian of the semi- conductor with the quantum共possibly inhomogeneous兲 light field and the interaction Hamiltonian of excitons with the phonon bath determining inelastic scattering and dephasing.

^{9}The kinetic equation for diagonal terms of the exciton den-

a兲Author to whom correspondence should be addressed; electronic mail:

pistone@unime.it

*sity matrix N*_{␣}⫽具^{B}^{ˆ}_{␣}^{†}* ^{B}^{ˆ}*␣典 can be derived starting from the
Heisenberg equation of motion for the exciton operators un-

*der the influence of H. The main approximations are the*neglect of possible coherent phonon states and of memory effects induced by the photon and phonon fields. The result is

*t**N*_{␣}*⫽G*_{␣}共*I*兲⫹

### 兺

_{}

^{␥}

^{␣←}

^{N}^{}

^{⫺2⌫}

^{␣}

^{N}^{␣}

^{,}

^{共2兲}

where the resulting phonon-assisted scattering rates ␥*←␣*

are given by ␥*←␣*⫽(2^{/}ប^{2})兺**q***兩t*_{␣,}** ^{q}** 兩

^{2}

*关n(*

**q**)␦

_{␣,,q}^{⫹}⫹(1

*⫹n(***q**))␦**␣,,q**⫺ *兴, n(***q**) being the thermal phonon occupa-
tion functions and ␦**␣,,q**⫾ ⫽␦^{(}_{␣}⫺_{}⫾**q**). The scattering
*matrix elements t*_{␣,}** ^{q}** depend on the lattice deformation po-
tentials and the overlap between the exciton states.

^{9}2⌫

_{␣}

*⫽r*_{␣}⫹兺_{}␥_{←␣}*is the total out-scattering rate, r*_{␣} being the
rate for radiative recombination proportional to the exciton
*oscillator strength: r*_{␣}*⫽r*0*兩兰d*^{2}**R**_{␣}** ^{(R)}**兩

^{2}共we assume that the tip-sample interaction does not alter the radiative decay rates兲. In the above equation the generation term depends on

*the spatial overlap between the illuminating field E*

_{I}**(r) and**the exciton wave functions corresponding to exciton levels

*resonant with the input light: G*

_{␣}

**(R**

*)*

_{I}*⫽r*0

*兩o*

_{␣}

^{I}**(R**

*)兩*

_{I}^{2}

*L*

_{␣}(

*I*) with

*L*

_{␣}(

^{)}⫽⌫/关(⫺␣)

^{2}⫹⌫

^{2}兴 and

*o*

_{␣}

^{I}**(R**

*)*

_{I}*⫽兰d*^{2}**RE**˜_{I}**(R)**_{␣}**(R) where E**˜_{I}**(R)***⫽兰E**I** (r) f (z)dz. In the*
subsequent numerical calculations concerning the illumina-
tion mode we will assume an input light field with a given

**Gaussian profile centered around the tip position R**

*:*

_{I}*E˜*

_{I}**(R)**

*⫽E*

*I*

0**g(R****⫺R***I*). In this case the generation term be-
comes function of the beam position and shape共spatial reso-
lution兲.

Once the exciton densities have been derived, the fre-
quency integrated PL can be readily obtained. It results in
**I(R***C*)*⫽r*0兺_{␣}*兩o*_{␣}^{C}**(R*** _{C}*)兩

^{2}

*N*

_{␣}

*, where o*

_{␣}

^{C}*, analogously to o*

_{␣}

*, contains the overlap of the exciton wave functions with the*

^{I}*signal mode E˜*

_{C}**(R) delivered by the tip**共collection mode兲.

According to the quantum regression theorem,
具^{Sˆ}^{⫺}^{(0)Sˆ}^{⫹}^{(}^{)}典 has the same dynamics of 具^{Sˆ}^{⫹}^{(}^{)}典 共propor-
tional to the exciton operator兲, but with 具^{Sˆ}^{⫺}^{(0)Sˆ}^{⫹}^{(0)}典 ^{as}
initial condition. Following this procedure we obtain
**I(R***C*,*C*)*⫽r*0兺_{␣}*兩o*_{␣}^{C}**(R*** _{C}*)兩

^{2}

*L*

_{␣}(

*C*

*) N*

_{␣}.

We apply the above developed theoretical scheme to
analyze the spatially resolved light emission of a QD system
arising from interface fluctuations of GaAs QWs. The effec-
*tive disordered potential felt by 1s excitons used in our*
simulations is obtained summing up two different contribu-
tions, both modeled as a zero mean, Gauss distributed and
spatially correlated process. We used⫽16 nm 共the correla-
tion length*兲, v*0⫽1.5 meV 共the width of the energy distribu-
tion兲; and*⫽8 nm, v*0⫽0.5 meV, respectively.

Figure 1共a兲 displays the specific realization of the effec-
tive disordered potential used for all the calculations. Figures
1共b兲–1共d兲 show energy-integrated PL images obtained after
uniform illumination of the sample at energy *I*⫽1 meV
*共the zero of energy is fixed at the energy of the 1s exciton in*
absence of disorder兲 and collecting locally the emitted light
*关C mode with spatial resolution full width at half maximum*
共FWHM兲⫽47 nm兴. It is worth noting that the energy-
integrated excitonic local density of states does not depend
on position. So the observed structures are a direct conse-
quence of the increasing ratio between radiative and nonra-

diative scattering rates for exciton states localized at the po-
tential minima关compare, e.g., images 1共a兲 and 1共c兲兴. As the
temperature of the structure is lowered, a transition from a
broad and fairly continuous PL to an intense set of few spa-
tially localized luminescence centers can be observed. An-
other interesting feature is the nonmonotonous brightness of
some luminescence centers when the temperature is in-
creased 关see, e.g., the location indicated by an arrow in im-
age 1共b兲兴, due to excitons which can overcome shallow local
minima by thermal activation and fall down in still deeper
states.^{8}

In Fig. 2 we report the emission intensity as a function of
both the illumination and collection energy for the three
*main working modes of the SNOM: I* 共local illumination,
far-field collection*兲, C 共far-field illumination, local collec-*
tion*兲 and I-C mode 共both local illumination and collection兲.*

The tip 共a spatial resolution of FWHM⫽94 nm is assumed兲 for local illumination and/or detection is centered at the po-

FIG. 1. 共a兲. Specific realization of disorder potential; 共b兲–共d兲 energy-
integrated PL images obtained after uniform illumination of the sample at
energy*I*⫽1 meV and collecting locally the emitted light.

FIG. 2.共Color兲 Emission intensity as a function of both the illumination and
collection energy for the three main working modes of the SNOM. A small
region along the diagonal (*C*⫽*I*) containing strong elastic contributions
is canceled.

sition indicated by a circle in Fig. 1共a兲. Figure 2 clearly
shows the impact that the specific working mode of the in-
*strument can have on the obtained results. The I-C images*
are the most selective and show a series of discrete peaks
that merge into quasicontinua 共corresponding to less local-
ized exciton states*兲 at higher energy, whereas the I mode is*
selective only for photoluminescence excitation 共PLE兲 mea-
surements (*C*fixed,*I*tuned*兲. On the contrary, the C mode*
shows good selectivity for PL measurements (*C* tuned,*I*

fixed兲, being of poor selectivity for PLE. This picture can be
better pointed out by looking at the sections of these gray-
scale plots shown in Fig. 3. Panel 3共a兲 displays for reference
the far-field and local absorption spectra. Figure 3共b兲 shows
*that the C and I-C modes give the same results when the*
sample is excited at quite a high energy and *C* is tuned.

*Also, the I and I-C modes almost coincide* 关see Fig. 3共c兲兴
when*C*is fixed at a low energy absorption peak. However,
Fig. 3共d兲 shows that in other circumstances the three working
modes produce different results. It is also interesting to no-
tice the differences in the peaks height between PLE and
local absorption spectra. The strong nonequivalence between
different SNOM kinds, here observed, is consequence共and at
the same time a direct proof兲 of the nonlocal nature of the
incoherent energy transfer between different regions of the
sample involving length scales significantly larger than

SNOM spatial resolutions 共even in presence of well defined dots兲. Further evidence is given by the strong differences between the calculated local absorption and emission spectra in some working mode. Finally, we note the thermal activa- tion of light up-conversion due to phonon-assisted exciton scattering clearly visible in the lower panels of Fig. 2.

In summary we have presented a microscopic quantum theory of spatially resolved photoluminescence in quantum wells with interface fluctuations. The theory establishes a clear functionality of the different SNOM kinds when ap- plied to the analysis of semiconductor quantum structures.

Moreover, this formulation permits one to model PL excita- tion spectroscopy in which the excitation and detection en- ergies and spatial positions can all independently be scanned.

The numerical results here presented constitute an intriguing example of the impact of sample temperature, exciton local- ization, and microscope setup in the formation of subwavelength-resolution images.

1H. F. Hess, E. Betzig, T. D. Harris, L. N. Pfeiffer, and K. W. West, Science
**264, 1740**共1994兲.

2**D. Gammon, E. S. Snow, and D. S. Katzer, Appl. Phys. Lett. 67, 2391**
共1995兲.

3D. Gammon, E. S. Snow, B. V. Shanabrook, D. S. Katzer, and D. Park,
**Phys. Rev. Lett. 76, 3005****共1996兲; Science 273, 87 共1996兲.**

4**Q. Wu, R. D. Grober, D. Gammon, and D. S. Katzer, Phys. Rev. Lett. 83,**
2652共1999兲.

5J. Hasen, L. N. Pfeiffer, A. Pinczuk, S. He, K. W. West, and B. S. Dennis,
Nature**共London兲 390, 54 共1997兲.**

6**S.-K. Eah, W. Jhe, and Y. Arakawa, Appl. Phys. Lett. 80, 2779**共2002兲.

7A. Zrenner, L. V. Butov, M. Hagn, G. Abstreiter, G. Bo¨hm, and G. We-
**imann, Phys. Rev. Lett. 72, 3382**共1994兲.

8**R. Zimmermann and E. Runge, Phys. Status Solidi A 164, 511**共1997兲.

9*R. Zimmermann, E. Runge, and S. Savona, in Quantum Coherence, Cor-*
*relation and Decoherence in Semiconductor Nanostructures, edited by T.*

Takagahara共Elsevier, New York, 2003兲, pp. 89–165.

10**O. Mauritz, G. Goldoni, F. Rossi, and E. Molinari, Phys. Rev. Lett. 82,**
847共1999兲.

11O. Di Stefano, S. Savasta, G. Martino, and R. Girlanda, Appl. Phys. Lett.

**77, 2804**共2000兲.

12**O. Di Stefano, S. Savasta, and R. Girlanda, J. Appl. Phys. 91, 2302**共2002兲.

13**G. Pistone, S. Savasta, O. Di Stefano, and R. Girlanda, Phys. Rev. B 67,**
153305共2003兲.

14**E. R. Mendez, J.-J. Greffet, and R. Carminati, Opt. Commun. 142, 7**
共1997兲.

15**J.-J. Greffet and R. Carminati, Prog. Surf. Sci. 56, 133**共1997兲.

16M. Pieruccini, S. Savasta, R. Girlanda, R. C. Iotti, and F. Rossi, Appl.

**Phys. Lett. 83, 2480**共2003兲.

17**V. M. Axt, K. Victor, and A. Stahl, Phys. Rev. B 53, 7244**共1996兲.

FIG. 3. 共a兲 Far-field spectrum and local absorption spectrum calculated
centering the tip at the position indicated by a circle in Fig. 1共a兲. 共b兲,共c兲,共d兲
Line scans共PL and PLE spectra兲 indicated by the letters 共b,c,d兲 in Fig. 2 for
*the three different working modes (T*⫽10^{0}K).